### Physics and Astronomy Publications

### Physics and Astronomy

### 6-2000

## Evidence for a strong impact of the electron-photon

## matrix element on angle-resolved photoelectron

## spectra of layered cuprate compounds

### S. Haffner

*Iowa State University*

### C. G. Olson

*Iowa State University*

### L. L. Miller

*Iowa State University*

### David W. Lynch

*Iowa State University*, dlynch@iastate.edu

### Follow this and additional works at:

### http://lib.dr.iastate.edu/physastro_pubs

### Part of the

### Atomic, Molecular and Optical Physics Commons

### , and the

### Condensed Matter

### Physics Commons

The complete bibliographic information for this item can be found athttp://lib.dr.iastate.edu/physastro_pubs/99. For information on how to cite this item, please visithttp://lib.dr.iastate.edu/howtocite.html.

### Evidence for a strong impact of the electron-photon matrix element on

### angle-resolved photoelectron spectra of layered cuprate compounds

**Abstract**

### Little is known about the impact of the electron-photon matrix element on angle-resolved photoelectron

### spectra of layered cuprate compounds. Using the example of the model layered cuprate Sr2CuO2Cl2, we

### demonstrate that the electron-photon matrix element has a significant influence on energy distribution

### curves, rendering their interpretation as images of the spectral function nontrivial.

**Keywords**

### Ames Laboratory, ARPES, one-electron Green’s function

**Disciplines**

### Atomic, Molecular and Optical Physics | Condensed Matter Physics | Physics

**Comments**

### This article is from

*Physical Review B*

### 61 (2000): 14378, doi:10.1103/PhysRevB.61.14378. Posted with

### permission,

**Evidence for a strong impact of the electron-photon matrix element on angle-resolved**

**photoelectron spectra of layered cuprate compounds**

S. Haffner, C. G. Olson, L. L. Miller, and D. W. Lynch

*Department of Physics and Astronomy and Ames Laboratory, U.S. Department of Energy, Iowa State University, Ames, Iowa 50011*

共Received 26 January 2000兲

Little is known about the impact of the electron-photon matrix element on angle-resolved photoelectron spectra of layered cuprate compounds. Using the example of the model layered cuprate Sr2CuO2Cl2, we demonstrate that the electron-photon matrix element has a significant influence on energy distribution curves, rendering their interpretation as images of the spectral function nontrivial.

Angle-resolved photoelectron spectroscopy 共ARPES兲 has played an important role in the study of layered cuprate com-pounds such as, for example, the high-temperature supercon-ductors. Examples of results obtained by ARPES are the ex-istence of a Fermi surface in the normal state compatible with the Luttinger theorem1–3and the observation of the su-perconducting gap and its anisotropy as well as a gap in the normal state in the underdoped regime.4–6One of the appeal-ing features of ARPES is that the spectral intensity of an electron distribution curve共EDC兲 is directly proportional to the electron-photon matrix element weighted spectral function.7Direct insight into the spectral function can there-fore be gained, which currently is not possible with any other experimental method. ARPES also allows a direct compari-son to theoretical models, as the spectral function is directly proportional to the imaginary part of the one-electron Green’s function of many-body theory.8

Nonetheless, one has to stress that the spectral intensity
observed in an EDC is proportional to the electron-photon
matrix element weighted spectral function and not the
spec-tral function itself. In most studies the influence of the matrix
element on an EDC is ignored although calculations suggest
that the relationship between ARPES intensities and the
un-derlying electronic structure can be quite complicated due to
matrix element effects, and that caution should be exercised
in interpreting detailed features of the ARPES intensities in
terms of the spectral function.9In the following, using
angle-resolved photoelectron spectra of Sr2CuO2Cl2 as an
ex-ample, it will be experimentally demonstrated that for
lay-ered cuprates the electron-photon matrix element can have a
*significant impact on both the relative spectral intensity and*
the shape of a feature in an ARPES spectrum.

Before discussing our results in detail, some information
about Sr2CuO2Cl2relevant for an understanding of this study
is given. Sr2CuO2Cl2 was chosen as it can be regarded as a
model system for the physics of layered cuprates having
CuO2 planes as their fundamental building block.
Sr_{2}CuO_{2}Cl_{2} is closely related to the undoped parent
com-pounds of the high-temperature superconductors as it is also
an antiferromagnetic insulator having a Ne´el temperature of
255 K.10The CuO2 planes in Sr2CuO2Cl2are undoped共half
filling兲; therefore the spectral intensity in an EDC related to
the CuO2 plane gives information about the dynamics of a
single hole 共the hole created by photoionization兲in a CuO_{2}

plane. The ARPES experiments in this study were performed
at 300 K. Although there is no long-range antiferromagnetic
order at room temperature in Sr_{2}CuO_{2}Cl_{2}, the
antiferromag-netic correlation length is still two orders of magnitude larger
than the Cu-O distance.10Therefore photoemission, as a fast
and local probe, still registers the effect of antiferromagnetic
order even 50 K above the Ne´el temperature.11

The dynamics of a hole in a two-dimensional
antiferro-magnetic background is of fundamental interest itself and
there have been numerous theoretical12 and
experimental11,13–16studies of this subject. Of primary
inter-est here are the lowinter-est-lying states in an ARPES spectrum,
the so-called first electron-removal states, which, according
to most theoretical results, should be comprised of a
low-binding-energy quasiparticle peak ascribed to the so-called
Zhang-Rice singlet17 共ZRS兲followed by incoherent spectral
weight at higher binding energy due to quasiparticle
dressing.12 The first electron-removal states of Sr2CuO2Cl2
indeed show a well-developed low-binding-energy peak
fol-lowed by additional spectral weight at higher binding
**ener-gies for k vectors along the**⌫ to (,) direction of the first
Brillouin zone 共BZ兲 of the CuO2 plane.18 In this work we
will not further elaborate on the physics behind the first
electron-removal states of Sr2CuO2Cl2 but rather use them
for a study of the impact of the electron-photon matrix
ele-ment on ARPES spectra of layered cuprates. They are
well-suited models for this, since there are no complications due
to apical oxygen atoms as in La2⫺*x*Sr*x*CuO4, no states
de-rived from Cu-O chains as in YBa_{2}Cu_{3}O* _{x}*, no superstructure
effects as in Bi2Sr2CaCu2O8 共BSCCO兲, and, finally, no
Fermi energy cutoffs due to their insulating nature.

The angle-resolved photoelectron spectra were recorded
on the storage ring Aladdin at the University of
Wisconsin-Madison Synchrotron Radiation Center, on the Ames
Laboratory/Montana State University ERG/SEYA beamline
using a 50 mm radius hemispherical analyzer having a 2 °
**full angular acceptance angle which corresponds to a k **
reso-lution of 0.06 Å⫺1 and 0.1 Å⫺1 关5% and 9% of the
dis-tance between ⌫ and (,)兴 for the first electron-removal
states and 22 eV and 35 eV photon energy, respectively. The
total energy resolution was 105 meV and 115 meV for 22 eV
and 35 eV photons, respectively. The angle of incidence of
the photons was ⬃40 ° with respect to the sample surface
normal. The Sr2CuO2Cl2 single crystal was grown as
de-PHYSICAL REVIEW B VOLUME 61, NUMBER 21 1 JUNE 2000-I

PRB 61

scribed elsewhere.19 *The sample was oriented ex situ by*
Laue backscattering and mounted with the Cu-O oxygen
bonds in a horizontal/vertical plane. The sample was cleaved

共cleavage plane parallel to CuO2 planes兲in the experimental
chamber in a vacuum better than 6⫻10⫺11 Torr, and the
*sample alignment was confirmed in situ by using the *
sym-metry of the dispersion of spectral features at high-symsym-metry
points. All EDC’s were recorded at room temperature and
were normalized to the photon flux. The Fermi edge of a
platinum foil in electrical contact with the sample was used
as binding energy reference. There were no indications of
**charging effects because repeating an EDC for a k point after**
the beam had decayed to less than half the current when the
first EDC was taken gave the same EDC, except for signal
strength. All ARPES spectra shown in this contribution were
recorded within a time of 28 hours after the cleave of the
sample and in one experimental run, i.e., using the same
sample cleave. We observed no signs of sample degradation
during this span of time.

Figure 1 presents the first electron-removal states of
Sr2CuO2Cl2**for k vectors along the**⌫to (,) and the⌫ to
(**,0) directions in k space recorded using 22 eV photon**
**energy. For k vectors from**⌫ to (,) we observe a distinct
low-energy peak whose peak maximum has its lowest
bind-ing energy (⬃0.84 eV) at ⬃(/2,/2) and the majority of
**its spectral intensity for k vectors before (**/2,/2). Along⌫
to (,0) there is a broad peak at ⬃1.1-1.2 eV binding
**en-ergy, which can only be observed in a range of k vectors**
from⬃50% to⬃85% of the distance between⌫ and (,0)
and has its maximum spectral intensity at⬃70% of the
dis-tance between ⌫ and (,0). These results are in agreement

with all previous studies of the first electron-removal states of Sr2CuO2Cl2,11,13and the closely related Ca2CuO2Cl2,14,15 which were recorded at about the same photon energy

共22–25 eV兲as the spectra shown in Fig. 1. This is no longer the case if we look at the first electron-removal states along

⌫ to (,) recorded using 35 eV photon energy, which are
shown in Fig. 2. It is evident that there are differences
be-tween the 22 eV and the 35 eV⌫to (,) series of ARPES
spectra, for example, in the relative strength of the peak as a
**function of k. In Fig. 2 there is no well-developed peak at**
(/2,**/2) but only for k vectors between (0.26**,0.26)
and (0.43,0.43), while in the left panel of Fig. 1 a distinct
peak is observed from (0.29,0.29) up to (0.58,0.58).
But, most notably, there are also differences in the line
shape, which are reflected in the dispersion of the peak
maxima presented in Fig. 3. While the dispersion relation
deduced from the 22 eV data peaks at⬃50% of the distance
between⌫ and (,), the peak in the 35 eV data set has its
minimum binding energy at ⬃(0.39,0.39). From theory
it is expected that the ZRS has its minimum binding energy
along ⌫ to (,) at (/2,/2).12 In the following we will
discuss possible reasons for the observed differences
be-tween the 22 eV and 35 eV ARPES data along the ⌫ to
(,**) direction in k space and show that our Sr**2CuO2Cl2
ARPES data can be understood only in terms of a strong
impact of matrix element effects on the EDC.

We can exclude the possibility that the observed
differ-ences are related to the sample or an extraordinary cleave of
the sample, as our 35 eV data are recorded using the same
sample and the same cleave as was used for the 22 eV data,
which, as mentioned earlier, are in agreement with all
previ-ously published Sr_{2}CuO_{2}Cl_{2} ARPES results recorded for
22–25 eV photon energy. This also excludes, besides our
experimental precautions, the possibility of a misalignment

FIG. 1. Sr2CuO2Cl2 ARPES spectra recorded along the ⌫ to
(,) direction 共left panel兲 and the ⌫ to (,0) direction 共right
panel兲**of the first BZ using 22 eV photon energy. The k vectors are**
given in % of the distance between⌫ and (,)/(,0).

FIG. 2. Sr2CuO2Cl2 ARPES spectra recorded along the ⌫ to
(,**) direction of the first BZ using 35 eV photon energy. The k**
vectors are given in % of the distance between⌫ and (,).

of the sample. Charging can shift spectral intensity to higher
binding energy and severely distort spectra, so one could
argue that the fact that in the 35 eV ARPES spectra the peak
maximum shifts back to higher binding energy before
(/2,**/2) and also the lack of a distinct peak at k vectors**
where one is observed in the 22 eV data are caused by
charg-ing. But note that the maximum photon flux during recording
of the 35 eV ARPES spectra was still six times lower than
the minimum photon flux during recording of the 22 eV data,
so we would then expect to observe such effects in the 22 eV
ARPES spectra too, which is not the case.

From the foregoing discussion we can conclude that the
spectra shown in Fig. 1 and in Fig. 2 truly represent the
low-binding-energy ARPES response of Sr2CuO2Cl2 for 22
or 35 eV photon energy, respectively. Both ⌫ to (,)
se-ries of EDC’s are equivalent in the sense that they show the
lowest-lying excitations associated with the motion of a hole
in an antiferromagnetically ordered CuO2**plane for k vectors**
along the ⌫ to (,) direction in the first BZ, i.e., the
un-derlying spectral function is the same. The two series of
EDC’s differ, however, in the photoelectron momentum
**vec-tor p and the final state**兩*f*

### 典

and maybe also the initial state### 具

*i*兩

共see the next paragraph兲of the photoexcitation process, both factors that affect the electron-photon matrix element

### 具

*i*兩

**p**•

**A**兩

*f*

### 典

共**where A is the vector potential**兲. As the underlying spectral function is the same in both cases, this suggests that the electron-photon matrix element is the reason for the ob-served differences.

The question remains how strongly the electron-photon
matrix element influences the EDC’s. One possibility is that
we see different initial states dependent on, for example,
photon energy but with the shape of the corresponding
fea-tures in the ARPES spectra and their relative intensities as a
**function of k being representative for the spectral function.**
In this case we have to explain the differences between the
22 eV and the 35 eV ⌫ to (,) spectra by assuming that
the peak observed in the 22 eV spectra has a different

physi-cal origin from the peak observed in the 35 eV data. But, as
mentioned earlier, up to now most authors have ascribed the
peak evident in the first electron-removal states of
Sr2CuO2Cl2 or Ca2CuO2Cl2to one excitation, the ZRS. It is
also not possible that we observe only the coherent part of
the spectral function of the ZRS for, for example, 22 eV and
the incoherent part for 35 eV as both share a common matrix
element. It has been suggested that a hole in an
antiferromag-netically ordered Cu-O plane can decay into spinons and
holons as is the case in one dimension.20 But the spectral
function predicted by the ‘‘two-dimensional spinon-holon
model’’ does not show different peaks for the spinon and the
holon, but only one peak due to an attractive spinon-holon
**interaction for k vectors from** ⌫ to (,) and a steplike
**feature for k vectors from**⌫to (,0), in contradiction to the
experimentally observed broad peak 共see the right panel of
Fig. 1兲. We have to conclude that according to current
knowledge the first electron-removal states of Sr2CuO2Cl2
have to be assigned to a ZRS, i.e., one initial state.

It should be evident now that there is no way to
under-stand the differences between the 22 eV and 35 eV ⌫ to
(,) ARPES spectra in the relative spectral intensities of
**the ZRS peak as a function of k without at least assuming**
that the relative intensity of the ZRS peak in the spectra is
strongly affected by the electron-photon matrix element.
This is also in agreement with the previously mentioned
the-oretical results of Ref. 9 for the ARPES intensities of
BSCCO. It remains to be clarified why the shape of the
EDC’s of the first electron-removal states of Sr2CuO2Cl2 is
**different for a given k vector using 22 eV or 35 eV photon**
energy, which also leads to differences in the dispersion
re-lations deduced from the spectra 共Fig. 3兲.

Let us first discuss some possible reasons for this effect
that would not be related to the electron-photon matrix
ele-ment. First, it could be argued that the peak dispersion could
be dependent on the momentum component perpendicular to
the cleavage plane. But it should be emphasized that for a
ZRS it is not expected that its dispersion will be dependent
on the momentum component perpendicular to the CuO_{2}
planes 共parallel to the cleavage plane兲.12 Another reason
could be the background as the ZRS peak is on top of a
steplike feature which is also observed in the ARPES spectra
of the high-temperature superconductors and whose origin is
currently unknown. This steplike feature could influence the
shape and the position of maximum intensity of the peak
ascribed to the ZRS. But judging from spectra where there is
no ZRS peak present, there seems not to be a lot of change of
the shape of this background on going from⌫ to (,) for
**the 22 eV or for the 35 eV data. The k-dependent change of**
the location of the maximum of the ZRS peak should
there-fore not be influenced significantly by the background.

On the other hand, there is an explanation of the
differ-ences in line shape and dispersion of the Sr2CuO2Cl2 22 eV
and 35 eV ARPES spectra along ⌫ to (,) if one accepts
that the electron-photon matrix element can influence the
shape of an individual EDC. Note that both dispersion
**rela-tions are equal within the error bars up to the k vector after**
which the ZRS peak in the 35 eV ARPES spectra loses most
**of its intensity. It is only after this point in k space that the**
dispersion relations deduced from the⌫to (,) 22 eV and
35 eV ARPES spectra differ. This suggests that the observed
differences in line shape and dispersion are caused by the

**FIG. 3. Binding energy of the ZRS peak as a function of k for k**
vectors from⌫ to (,) deduced from the spectra recorded at 22
eV共solid circles兲and 35 eV共open circles兲photon energy. Selected
error bars are shown for reference.

electron-photon matrix element due to which the ZRS peak
in the 35 eV ARPES spectra may be cut after
(0.39,0.39), thus not only losing intensity but also having
the maximum of the spectral intensity shifted to higher
bind-ing energy, leadbind-ing to an apparent dispersion that is different
from that of the ZRS peak in the spectral function. An
influ-ence of the electron-photon matrix element on the shape of
an ARPES spectrum was not reported for the calculated
BSSCO ARPES response of Ref. 9. A possible reason for
**this discrepancy could be the finite k resolution of our**
ARPES experiment, which in conjunction with possibly
sig-nificantly different dispersion relations of the final states
reached using 22 eV and 35 eV photons could lead to a
different shape of the 22 eV and 35 eV spectra for the same
**k vector. Another reason could be that the calculations were**
performed in the framework of the local-density
approxima-tion, which is generally not well suited to describe either the
lowest-lying occupied band of a layered cuprate or the final
states 15 eV and more above the Fermi level.

In conclusion, we have observed that the electron-photon matrix element can have a profound impact on ARPES spec-tra of layered cuprates by significantly affecting the strength

*and the shape of spectral features. The results of this study*

clearly put emphasis on the need to apply the whole
param-eter range of the ARPES technique in order to get reliable,
consistent, and complete information about the spectral
func-tion from an ARPES experiment. This is especially
impor-tant when one has to rely on ARPES spectral intensities as is
the case in an analysis of the momentum distribution
function7,15 * n(k)* 共the momentum-integrated spectral
inten-sity兲and in the angle-scanning mode of angle-resolved
pho-toelectron spectroscopy.21

The Ames Laboratory is operated by Iowa State Univer-sity for the U.S. DOE under Contract No. W-7405-ENG-82. This work is based upon research conducted at the Synchro-tron Radiation Center, University of Wisconsin, Madison, which is supported under Award No. DMR-95-31009.

1_{C. G. Olson, R. Liu, D. W. Lynch, R. S. List, A. J. Arko, B. W.}

Veal, Y. C. Chang, P. Z. Jiang, and A. P. Paulikas, Phys. Rev. B
**42, 381**共1990兲.

2_{J. C. Campuzano, G. Jennings, M. Faiz, L. Beaulaigue, B. W.}

Veal, J. Z. Liu, A. P. Paulikas, K. Vandervoort, and H. Claus,
**Phys. Rev. Lett. 64, 2308**共1990兲.

3_{R. O. Anderson, R. Claessen, J. W. Allen, C. G. Olson, C. }

Jan-owitz, L. Z. Liu, J.-H. Park, M. B. Maple, Y. Daliachouch, M.
C. de Andrade, R. F. Jardim, E. A. Early, S.-J. Oh, and W. P.
**Ellis, Phys. Rev. Lett. 70, 3163**共1993兲.

4_{C. G. Olson, R. Liu, A.-B. Yang, D. W. Lynch, A. J. Arko, R. S.}

List, B. W. Veal, Y. C. Chang, P. Z. Jiang, and A. P. Paulikas,
**Science 245, 731**共1989兲.

5

Z.-X. Shen, D. S. Dessau, B. O. Wells, D. M. King, W. E. Spicer,
A. J. Arko, D. Marshall, L. W. Lombardo, A. Kapitulnik, P.
Dickinson, S. Doniach, J. DiCarlo, A. G. Loeser, and C. H. Park,
**Phys. Rev. Lett. 70, 1553**共1993兲.

6_{D. S. Marshall, D. S. Dessau, A. G. Loeser, C.-H. Park, A. Y.}

Matsuura, J. N. Eckstein, I. Bozovic, P. Fournier, A. Kapitulnik,
**W. E. Spicer, and Z.-X. Shen, Phys. Rev. Lett. 76, 4841**共1996兲.
7_{M. Randeria, H. Ding, J.-C. Campuzano, A. Bellman, G. }

Jen-nings, T. Yokoya, T. Takahashi, H. Katayama-Yoshida, T.
**Mo-chiku, and K. Kadowaki, Phys. Rev. Lett. 74, 4951**共1995兲.
8_{S. Huefner, Photoelectron Spectroscopy}_{共}_{Springer, Berlin, 1995}_{兲}_{.}
9_{A. Bansil and M. Lindroos, J. Phys. Chem. Solids 59, 1879}

共1998兲.

10_{M. Greven, R. J. Birgeneau, Y. Endoh, M. A. Kastner, B. Keimer,}

M. Matsuda, G. Shirane, and T. R. Thurston, Phys. Rev. Lett.
**72, 1096**共1994兲.

11_{B. O. Wells, Z.-X. Shen, A. Matsuura, D. M. King, M. A. }

**Kast-ner, M. Greven, and R. J. Birgeneau, Phys. Rev. Lett. 74, 964**

共1995兲.

12_{E. Dagotto, Rev. Mod. Phys. 66, 763}_{共}_{1994}_{兲}_{.}

13_{S. LaRosa, I. Vobornik, F. Zwick, H. Berger, M. Grioni, G. }

Mar-garitondo, R. J. Kelley, M. Onellion, and A. Chubukov, Phys.
**Rev. B 56, R525**共1997兲.

14_{C. Kim, P. J. White, Z.-X. Shen, T. Tohyama, Y. Shibata, S.}

Maekawa, B. O. Wells, Y. J. Kim, R. J. Birgeneau, and M. A.
**Kastner, Phys. Rev. Lett. 80, 4245**共1998兲.

15_{F. Ronning, C. Kim, D. L. Feng, D. S. Marshall, A. G. Loeser, L.}

L. Miller, J. N. Eckstein, I. Bozovic, and Z.-X. Shen, Science
**282, 2067**共1998兲.

16_{M. S. Golden, H. C. Schmelz, M. Knupfer, S. Haffner, G. }

Krab-bes, J. Fink, V. Y. Yushankhai, H. Rosner, R. Hayn, A. Mueller,
**and G. Reichardt, Phys. Rev. Lett. 78, 4107**共1997兲.

17_{F. C. Zhang and T. M. Rice, Phys. Rev. B 37, 3759}_{共}_{1988}_{兲}_{.}
18_{k vectors are given in units of the inverse lattice constant of the}

CuO2plane.

19_{L. L. Miller, X. L. Wang, S. X. Wang, C. Stassis, D. C. Johnston,}

**J. Faber, Jr., and C.-K. Loong, Phys. Rev. B 41, 1921**共1990兲.
20_{R. B. Laughlin, J. Phys. Chem. Solids 56, 1627}_{共}_{1995}_{兲}_{; Phys.}

**Rev. Lett. 79, 1726**共1997兲.

21_{P. Aebi, J. Osterwalder, R. Fasel, D. Naumovic, and L. }

**Schlap-bach, Surf. Sci. 307-309, 917**共1994兲.